#------------------------------------------------------------------------------
#$Date: 2016-03-26 20:45:27 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180447 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/16/7211648.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7211648
loop_
_publ_author_name
'Zang, Hong-Ying'
'Lan, Ya-Qian'
'Yang, Guang-Sheng'
'Wang, Xin-Long'
'Shao, Kui-Zhan'
'Xu, Guang-Juan'
'Su, Zhong-Min'
_publ_section_title
;
 Construction and property investigation of transition-metal complexes
 modified octamolybdate hybrid materials based on V-shaped organic ligands
;
_journal_issue                   2
_journal_name_full               CrystEngComm
_journal_page_first              434
_journal_paper_doi               10.1039/b911881k
_journal_volume                  12
_journal_year                    2010
_chemical_formula_moiety         'C16 H16 Cl Cu3 Mo4 N8 O13'
_chemical_formula_sum            'C16 H16 Cl Cu3 Mo4 N8 O13'
_chemical_formula_weight         1138.20
_chemical_name_systematic
;
?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                96.116(3)
_cell_angle_beta                 102.112(3)
_cell_angle_gamma                108.448(4)
_cell_formula_units_Z            2
_cell_length_a                   10.651(3)
_cell_length_b                   11.293(3)
_cell_length_c                   12.834(7)
_cell_measurement_reflns_used    'total reflection'
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      26.04
_cell_measurement_theta_min      1.33
_cell_volume                     1406.7(9)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SMART'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.977
_diffrn_measured_fraction_theta_max 0.977
_diffrn_measurement_device_type  'Bruker SMART APEX II CCD area-detector'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0177
_diffrn_reflns_av_sigmaI/netI    0.0408
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            6985
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.65
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    4.122
_exptl_absorpt_correction_T_max  0.316
_exptl_absorpt_correction_T_min  0.208
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    2.687
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1088
_exptl_crystal_size_max          0.4
_exptl_crystal_size_mid          0.36
_exptl_crystal_size_min          0.28
_refine_diff_density_max         1.209
_refine_diff_density_min         -3.255
_refine_diff_density_rms         0.234
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.072
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     406
_refine_ls_number_reflns         4852
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.072
_refine_ls_R_factor_all          0.0743
_refine_ls_R_factor_gt           0.0615
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1125P)²+12.3739P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1768
_refine_ls_wR_factor_ref         0.1887
_reflns_number_gt                3917
_reflns_number_total             4852
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b911881k.txt
_cod_data_source_block           5
_cod_original_sg_symbol_H-M      p-1
_cod_database_code               7211648
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Cu1 Cu -0.3378(2) 1.32158(19) 1.48890(15) 0.0697(6) Uani 1 1 d .
Cu2 Cu -0.3775(3) 1.4927(3) 1.0778(2) 0.1025(9) Uani 1 1 d .
Cu3 Cu 0.12105(16) 1.13291(15) 1.01694(13) 0.0452(4) Uani 1 1 d .
Mo1 Mo 0.22293(9) 1.28325(9) 0.41920(8) 0.0309(3) Uani 1 1 d .
Mo2 Mo 0.16540(8) 0.98922(8) 0.50199(6) 0.0202(2) Uani 1 1 d .
Mo3 Mo -0.10028(9) 0.75480(8) 0.36789(7) 0.0270(3) Uani 1 1 d .
Mo4 Mo 0.05618(9) 0.95761(8) 0.71557(6) 0.0228(2) Uani 1 1 d .
C1 C 0.3150(13) 0.9978(13) 1.0156(10) 0.043(3) Uani 1 1 d .
H1 H 0.2907 0.9767 0.9403 0.051 Uiso 1 1 calc R
C2 C 0.3179(12) 1.0765(11) 1.1743(9) 0.037(3) Uani 1 1 d .
H2 H 0.2995 1.1171 1.2332 0.044 Uiso 1 1 calc R
C3 C 0.5119(12) 1.0169(12) 1.2758(10) 0.044(3) Uani 1 1 d .
H3A H 0.5028 1.0645 1.3396 0.052 Uiso 1 1 calc R
H3B H 0.6047 1.0550 1.2694 0.052 Uiso 1 1 calc R
C4 C 0.4860(11) 0.8801(11) 1.2888(9) 0.035(2) Uani 1 1 d .
C5 C 0.5211(12) 0.7955(12) 1.2240(10) 0.043(3) Uani 1 1 d .
H5 H 0.5616 0.8195 1.1684 0.051 Uiso 1 1 calc R
C6 C 0.4932(13) 0.6757(13) 1.2458(11) 0.047(3) Uani 1 1 d .
H7 H 0.5177 0.6173 1.2053 0.057 Uiso 1 1 calc R
C7 C 0.4312(15) 0.6393(13) 1.3243(11) 0.050(3) Uani 1 1 d .
H6 H 0.4111 0.5556 1.3344 0.061 Uiso 1 1 calc R
C8 C 0.4235(12) 0.8391(11) 1.3683(9) 0.037(3) Uani 1 1 d .
H8 H 0.3981 0.8957 1.4099 0.044 Uiso 1 1 calc R
C9 C -0.3771(13) 1.3726(11) 1.2713(11) 0.044(3) Uani 1 1 d .
H9 H -0.4701 1.3567 1.2629 0.053 Uiso 1 1 calc R
C10 C -0.1738(13) 1.3860(10) 1.3354(9) 0.037(3) Uani 1 1 d .
H10 H -0.0947 1.3836 1.3810 0.044 Uiso 1 1 calc R
C11 C -0.0733(12) 1.4634(11) 1.1881(10) 0.037(3) Uani 1 1 d .
H11A H 0.0135 1.4781 1.2395 0.045 Uiso 1 1 calc R
H11B H -0.0737 1.5446 1.1701 0.045 Uiso 1 1 calc R
C12 C -0.0844(11) 1.3756(10) 1.0862(9) 0.029(2) Uani 1 1 d .
C13 C -0.1584(12) 1.3778(11) 0.9847(10) 0.040(3) Uani 1 1 d .
H13 H -0.2104 1.4302 0.9774 0.048 Uiso 1 1 calc R
C14 C -0.1552(11) 1.3029(11) 0.8952(9) 0.036(3) Uani 1 1 d .
H14 H -0.2071 1.3025 0.8271 0.043 Uiso 1 1 calc R
C15 C -0.0759(10) 1.2289(10) 0.9057(8) 0.029(2) Uani 1 1 d .
H15 H -0.0733 1.1792 0.8441 0.035 Uiso 1 1 calc R
C16 C -0.0058(12) 1.2998(10) 1.0920(9) 0.033(2) Uani 1 1 d .
H16 H 0.0466 1.2988 1.1595 0.040 Uiso 1 1 calc R
N1 N 0.2521(10) 1.0618(9) 1.0732(7) 0.034(2) Uani 1 1 d .
N2 N 0.4123(11) 0.9699(12) 1.0778(8) 0.050(3) Uani 1 1 d .
N3 N 0.4166(9) 1.0243(9) 1.1812(8) 0.037(2) Uani 1 1 d .
N4 N 0.3975(12) 0.7197(11) 1.3883(8) 0.048(3) Uani 1 1 d .
N5 N -0.2973(12) 1.3613(9) 1.3589(8) 0.044(3) Uani 1 1 d .
N6 N -0.3145(10) 1.4083(10) 1.1961(8) 0.040(2) Uani 1 1 d .
N7 N -0.1844(9) 1.4132(8) 1.2398(7) 0.0293(19) Uani 1 1 d .
N8 N -0.0017(10) 1.2260(8) 1.0027(7) 0.032(2) Uani 1 1 d .
O1 O 0.1451(10) 1.3894(8) 0.3901(7) 0.053(2) Uani 1 1 d .
O2 O 0.3805(9) 1.3456(8) 0.3956(8) 0.048(2) Uani 1 1 d .
O3 O -0.2501(7) 0.6877(7) 0.4293(6) 0.0343(17) Uani 1 1 d .
O4 O 0.2826(7) 1.1115(7) 0.4640(6) 0.0297(16) Uani 1 1 d .
O5 O -0.1759(9) 0.7002(7) 0.2336(6) 0.0391(19) Uani 1 1 d .
O6 O 0.1811(7) 1.0751(6) 0.6462(5) 0.0246(14) Uani 1 1 d .
O7 O 0.2474(8) 0.8855(7) 0.5303(6) 0.0329(17) Uani 1 1 d .
O8 O -0.0042(9) 0.6649(7) 0.4028(7) 0.0405(19) Uani 1 1 d .
O9 O 0.0520(7) 0.9074(6) 0.3567(5) 0.0243(14) Uani 1 1 d .
O10 O -0.0280(6) 0.8843(6) 0.5338(5) 0.0219(14) Uani 1 1 d .
O11 O -0.1238(7) 0.8464(7) 0.7075(6) 0.0300(16) Uani 1 1 d .
O12 O 0.1483(8) 0.8617(7) 0.7402(6) 0.0323(16) Uani 1 1 d .
O13 O 0.0911(8) 1.0517(8) 0.8375(6) 0.0372(18) Uani 1 1 d .
Cl1 Cl -0.3628(5) 1.6136(5) 0.9589(4) 0.0889(14) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
N5 Cu1 N4 173.9(5) . 2_578
N6 Cu2 Cl1 158.1(4) . .
N6 Cu2 Cl1 100.3(3) . 2_487
Cl1 Cu2 Cl1 101.50(19) . 2_487
N6 Cu2 Cu2 145.0(4) . 2_487
Cl1 Cu2 Cu2 56.79(16) . 2_487
Cl1 Cu2 Cu2 44.71(14) 2_487 2_487
N1 Cu3 N8 163.5(4) . .
N1 Cu3 O13 96.0(3) . .
N8 Cu3 O13 100.5(3) . .
O1 Mo1 O2 104.9(5) . .
O1 Mo1 O3 98.5(4) . 2_576
O2 Mo1 O3 106.5(4) . 2_576
O1 Mo1 O11 98.3(4) . 2_576
O2 Mo1 O11 102.6(4) . 2_576
O3 Mo1 O11 141.1(3) 2_576 2_576
O1 Mo1 O4 167.2(4) . .
O2 Mo1 O4 87.9(3) . .
O3 Mo1 O4 78.5(3) 2_576 .
O11 Mo1 O4 77.3(3) 2_576 .
O7 Mo2 O4 104.7(4) . .
O7 Mo2 O9 100.6(3) . .
O4 Mo2 O9 96.6(3) . .
O7 Mo2 O6 101.9(3) . .
O4 Mo2 O6 98.5(3) . .
O9 Mo2 O6 148.6(3) . .
O7 Mo2 O10 98.1(3) . .
O4 Mo2 O10 157.2(3) . .
O9 Mo2 O10 78.1(3) . .
O6 Mo2 O10 77.3(3) . .
O7 Mo2 O10 173.1(3) . 2_576
O4 Mo2 O10 82.2(3) . 2_576
O9 Mo2 O10 77.8(2) . 2_576
O6 Mo2 O10 77.2(2) . 2_576
O10 Mo2 O10 75.0(3) . 2_576
O7 Mo2 Mo3 88.9(3) . .
O4 Mo2 Mo3 133.1(2) . .
O9 Mo2 Mo3 36.5(2) . .
O6 Mo2 Mo3 122.7(2) . .
O10 Mo2 Mo3 45.46(17) . .
O10 Mo2 Mo3 85.94(16) 2_576 .
O7 Mo2 Mo4 89.9(3) . .
O4 Mo2 Mo4 134.4(2) . .
O9 Mo2 Mo4 123.3(2) . .
O6 Mo2 Mo4 35.9(2) . .
O10 Mo2 Mo4 45.16(17) . .
O10 Mo2 Mo4 85.53(16) 2_576 .
Mo3 Mo2 Mo4 89.22(4) . .
O8 Mo3 O5 105.0(4) . .
O8 Mo3 O3 102.2(4) . .
O5 Mo3 O3 101.4(4) . .
O8 Mo3 O9 97.0(3) . .
O5 Mo3 O9 98.4(3) . .
O3 Mo3 O9 147.7(3) . .
O8 Mo3 O10 95.1(3) . .
O5 Mo3 O10 159.5(3) . .
O3 Mo3 O10 78.1(3) . .
O9 Mo3 O10 74.5(2) . .
O8 Mo3 O6 163.8(3) . 2_576
O5 Mo3 O6 88.0(3) . 2_576
O3 Mo3 O6 84.3(3) . 2_576
O9 Mo3 O6 71.1(2) . 2_576
O10 Mo3 O6 71.5(2) . 2_576
O8 Mo3 Mo2 85.2(3) . .
O5 Mo3 Mo2 133.6(3) . .
O3 Mo3 Mo2 120.9(2) . .
O9 Mo3 Mo2 35.22(18) . .
O10 Mo3 Mo2 42.81(16) . .
O6 Mo3 Mo2 78.83(17) 2_576 .
O12 Mo4 O13 104.1(4) . .
O12 Mo4 O11 101.5(3) . .
O13 Mo4 O11 100.0(4) . .
O12 Mo4 O6 97.2(3) . .
O13 Mo4 O6 99.9(4) . .
O11 Mo4 O6 148.4(3) . .
O12 Mo4 O10 97.1(3) . .
O13 Mo4 O10 158.6(3) . .
O11 Mo4 O10 78.5(3) . .
O6 Mo4 O10 74.0(3) . .
O12 Mo4 O9 166.0(3) . 2_576
O13 Mo4 O9 86.4(3) . 2_576
O11 Mo4 O9 85.5(3) . 2_576
O6 Mo4 O9 71.5(2) . 2_576
O10 Mo4 O9 72.2(2) . 2_576
O12 Mo4 Mo2 86.5(3) . .
O13 Mo4 Mo2 134.9(3) . .
O11 Mo4 Mo2 121.1(2) . .
O6 Mo4 Mo2 34.92(18) . .
O10 Mo4 Mo2 42.65(16) . .
O9 Mo4 Mo2 79.58(16) 2_576 .
N2 C1 N1 113.4(10) . .
N2 C1 H1 123.3 . .
N1 C1 H1 123.3 . .
N1 C2 N3 110.2(10) . .
N1 C2 H2 124.9 . .
N3 C2 H2 124.9 . .
N3 C3 C4 110.9(9) . .
N3 C3 H3A 109.5 . .
C4 C3 H3A 109.5 . .
N3 C3 H3B 109.5 . .
C4 C3 H3B 109.5 . .
H3A C3 H3B 108.1 . .
C8 C4 C5 119.3(11) . .
C8 C4 C3 117.5(11) . .
C5 C4 C3 123.1(11) . .
C6 C5 C4 116.8(11) . .
C6 C5 H5 121.6 . .
C4 C5 H5 121.6 . .
C7 C6 C5 121.9(12) . .
C7 C6 H7 119.0 . .
C5 C6 H7 119.0 . .
N4 C7 C6 122.2(12) . .
N4 C7 H6 118.9 . .
C6 C7 H6 118.9 . .
N4 C8 C4 122.6(11) . .
N4 C8 H8 118.7 . .
C4 C8 H8 118.7 . .
N5 C9 N6 114.1(11) . .
N5 C9 H9 122.9 . .
N6 C9 H9 122.9 . .
N7 C10 N5 108.9(10) . .
N7 C10 H10 125.5 . .
N5 C10 H10 125.5 . .
N7 C11 C12 113.2(9) . .
N7 C11 H11A 108.9 . .
C12 C11 H11A 108.9 . .
N7 C11 H11B 108.9 . .
C12 C11 H11B 108.9 . .
H11A C11 H11B 107.7 . .
C16 C12 C13 117.6(10) . .
C16 C12 C11 118.9(10) . .
C13 C12 C11 123.2(10) . .
C14 C13 C12 120.0(11) . .
C14 C13 H13 120.0 . .
C12 C13 H13 120.0 . .
C13 C14 C15 119.9(11) . .
C13 C14 H14 120.0 . .
C15 C14 H14 120.0 . .
N8 C15 C14 121.4(10) . .
N8 C15 H15 119.3 . .
C14 C15 H15 119.3 . .
N8 C16 C12 122.4(10) . .
N8 C16 H16 118.8 . .
C12 C16 H16 118.8 . .
C2 N1 C1 104.3(9) . .
C2 N1 Cu3 127.7(8) . .
C1 N1 Cu3 127.4(7) . .
C1 N2 N3 103.1(9) . .
C2 N3 N2 109.0(9) . .
C2 N3 C3 129.3(10) . .
N2 N3 C3 121.7(10) . .
C7 N4 C8 117.1(11) . .
C7 N4 Cu1 122.5(9) . 2_578
C8 N4 Cu1 120.0(9) . 2_578
C9 N5 C10 103.9(10) . .
C9 N5 Cu1 129.4(9) . .
C10 N5 Cu1 126.7(9) . .
C9 N6 N7 102.9(9) . .
C9 N6 Cu2 125.9(8) . .
N7 N6 Cu2 127.9(7) . .
C10 N7 N6 110.0(9) . .
C10 N7 C11 127.4(10) . .
N6 N7 C11 121.9(9) . .
C15 N8 C16 118.6(9) . .
C15 N8 Cu3 121.6(7) . .
C16 N8 Cu3 119.6(7) . .
Mo1 O3 Mo3 119.9(4) 2_576 .
Mo2 O4 Mo1 119.0(4) . .
Mo2 O6 Mo4 109.2(3) . .
Mo2 O6 Mo3 109.5(3) . 2_576
Mo4 O6 Mo3 105.0(3) . 2_576
Mo2 O9 Mo3 108.3(3) . .
Mo2 O9 Mo4 109.1(3) . 2_576
Mo3 O9 Mo4 105.0(3) . 2_576
Mo2 O10 Mo4 92.2(2) . .
Mo2 O10 Mo3 91.7(2) . .
Mo4 O10 Mo3 161.6(3) . .
Mo2 O10 Mo2 105.0(3) . 2_576
Mo4 O10 Mo2 97.9(2) . 2_576
Mo3 O10 Mo2 98.4(2) . 2_576
Mo4 O11 Mo1 119.7(4) . 2_576
Mo4 O13 Cu3 166.0(5) . .
Cu2 Cl1 Cu2 78.50(19) . 2_487
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cu1 N5 1.873(10) .
Cu1 N4 1.870(10) 2_578
Cu2 N6 1.987(10) .
Cu2 Cl1 2.151(6) .
Cu2 Cl1 2.559(6) 2_487
Cu2 Cu2 2.997(6) 2_487
Cu3 N1 1.878(9) .
Cu3 N8 1.913(9) .
Cu3 O13 2.303(7) .
Mo1 O1 1.690(8) .
Mo1 O2 1.707(8) .
Mo1 O3 1.882(8) 2_576
Mo1 O11 1.922(7) 2_576
Mo1 O4 2.315(7) .
Mo2 O7 1.694(7) .
Mo2 O4 1.735(7) .
Mo2 O9 1.942(7) .
Mo2 O6 1.943(7) .
Mo2 O10 2.174(6) .
Mo2 O10 2.361(7) 2_576
Mo2 Mo3 3.1972(13) .
Mo2 Mo4 3.2059(18) .
Mo3 O8 1.686(8) .
Mo3 O5 1.696(7) .
Mo3 O3 1.906(8) .
Mo3 O9 2.001(7) .
Mo3 O10 2.280(6) .
Mo3 O6 2.349(6) 2_576
Mo4 O12 1.688(7) .
Mo4 O13 1.693(7) .
Mo4 O11 1.905(7) .
Mo4 O6 1.989(7) .
Mo4 O10 2.275(6) .
Mo4 O9 2.340(6) 2_576
C1 N2 1.313(15) .
C1 N1 1.384(15) .
C1 H1 0.9300 .
C2 N1 1.304(14) .
C2 N3 1.351(14) .
C2 H2 0.9300 .
C3 N3 1.439(14) .
C3 C4 1.516(16) .
C3 H3A 0.9700 .
C3 H3B 0.9700 .
C4 C8 1.373(16) .
C4 C5 1.390(17) .
C5 C6 1.364(18) .
C5 H5 0.9300 .
C6 C7 1.348(19) .
C6 H7 0.9300 .
C7 N4 1.341(17) .
C7 H6 0.9300 .
C8 N4 1.352(15) .
C8 H8 0.9300 .
C9 N5 1.304(16) .
C9 N6 1.312(15) .
C9 H9 0.9300 .
C10 N7 1.288(14) .
C10 N5 1.360(16) .
C10 H10 0.9300 .
C11 N7 1.465(13) .
C11 C12 1.514(15) .
C11 H11A 0.9700 .
C11 H11B 0.9700 .
C12 C16 1.371(15) .
C12 C13 1.380(16) .
C13 C14 1.365(17) .
C13 H13 0.9300 .
C14 C15 1.361(15) .
C14 H14 0.9300 .
C15 N8 1.336(13) .
C15 H15 0.9300 .
C16 N8 1.361(14) .
C16 H16 0.9300 .
N2 N3 1.386(14) .
N4 Cu1 1.870(10) 2_578
N6 N7 1.362(13) .
O3 Mo1 1.882(8) 2_576
O6 Mo3 2.349(6) 2_576
O9 Mo4 2.340(6) 2_576
O10 Mo2 2.361(6) 2_576
O11 Mo1 1.922(7) 2_576
Cl1 Cu2 2.559(6) 2_487
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O7 Mo2 Mo3 O8 -0.3(4) . .
O4 Mo2 Mo3 O8 108.9(4) . .
O9 Mo2 Mo3 O8 109.4(4) . .
O6 Mo2 Mo3 O8 -103.8(4) . .
O10 Mo2 Mo3 O8 -102.8(4) . .
O10 Mo2 Mo3 O8 -175.8(3) 2_576 .
Mo4 Mo2 Mo3 O8 -90.2(3) . .
O7 Mo2 Mo3 O5 -106.4(4) . .
O4 Mo2 Mo3 O5 2.8(5) . .
O9 Mo2 Mo3 O5 3.3(5) . .
O6 Mo2 Mo3 O5 150.1(4) . .
O10 Mo2 Mo3 O5 151.1(4) . .
O10 Mo2 Mo3 O5 78.1(4) 2_576 .
Mo4 Mo2 Mo3 O5 163.7(4) . .
O7 Mo2 Mo3 O3 101.0(4) . .
O4 Mo2 Mo3 O3 -149.8(4) . .
O9 Mo2 Mo3 O3 -149.3(4) . .
O6 Mo2 Mo3 O3 -2.5(3) . .
O10 Mo2 Mo3 O3 -1.5(3) . .
O10 Mo2 Mo3 O3 -74.5(3) 2_576 .
Mo4 Mo2 Mo3 O3 11.1(3) . .
O7 Mo2 Mo3 O9 -109.7(4) . .
O4 Mo2 Mo3 O9 -0.5(4) . .
O6 Mo2 Mo3 O9 146.9(4) . .
O10 Mo2 Mo3 O9 147.8(4) . .
O10 Mo2 Mo3 O9 74.9(3) 2_576 .
Mo4 Mo2 Mo3 O9 160.4(3) . .
O7 Mo2 Mo3 O10 102.5(4) . .
O4 Mo2 Mo3 O10 -148.3(4) . .
O9 Mo2 Mo3 O10 -147.8(4) . .
O6 Mo2 Mo3 O10 -1.0(3) . .
O10 Mo2 Mo3 O10 -73.0(3) 2_576 .
Mo4 Mo2 Mo3 O10 12.6(2) . .
O7 Mo2 Mo3 O6 177.3(3) . 2_576
O4 Mo2 Mo3 O6 -73.5(4) . 2_576
O9 Mo2 Mo3 O6 -73.0(4) . 2_576
O6 Mo2 Mo3 O6 73.8(3) . 2_576
O10 Mo2 Mo3 O6 74.8(3) . 2_576
O10 Mo2 Mo3 O6 1.8(2) 2_576 2_576
Mo4 Mo2 Mo3 O6 87.40(17) . 2_576
O7 Mo2 Mo4 O12 2.8(3) . .
O4 Mo2 Mo4 O12 -107.8(4) . .
O9 Mo2 Mo4 O12 105.5(3) . .
O6 Mo2 Mo4 O12 -108.0(4) . .
O10 Mo2 Mo4 O12 104.4(4) . .
O10 Mo2 Mo4 O12 177.7(3) 2_576 .
Mo3 Mo2 Mo4 O12 91.7(3) . .
O7 Mo2 Mo4 O13 109.2(4) . .
O4 Mo2 Mo4 O13 -1.4(5) . .
O9 Mo2 Mo4 O13 -148.1(4) . .
O6 Mo2 Mo4 O13 -1.6(5) . .
O10 Mo2 Mo4 O13 -149.2(4) . .
O10 Mo2 Mo4 O13 -75.9(4) 2_576 .
Mo3 Mo2 Mo4 O13 -161.9(4) . .
O7 Mo2 Mo4 O11 -98.4(4) . .
O4 Mo2 Mo4 O11 150.9(4) . .
O9 Mo2 Mo4 O11 4.2(3) . .
O6 Mo2 Mo4 O11 150.8(4) . .
O10 Mo2 Mo4 O11 3.1(3) . .
O10 Mo2 Mo4 O11 76.5(3) 2_576 .
Mo3 Mo2 Mo4 O11 -9.5(3) . .
O7 Mo2 Mo4 O6 110.8(4) . .
O4 Mo2 Mo4 O6 0.2(4) . .
O9 Mo2 Mo4 O6 -146.5(4) . .
O10 Mo2 Mo4 O6 -147.6(4) . .
O10 Mo2 Mo4 O6 -74.3(4) 2_576 .
Mo3 Mo2 Mo4 O6 -160.3(3) . .
O7 Mo2 Mo4 O10 -101.6(4) . .
O4 Mo2 Mo4 O10 147.8(4) . .
O9 Mo2 Mo4 O10 1.1(3) . .
O6 Mo2 Mo4 O10 147.6(4) . .
O10 Mo2 Mo4 O10 73.3(3) 2_576 .
Mo3 Mo2 Mo4 O10 -12.7(2) . .
O7 Mo2 Mo4 O9 -176.6(3) . 2_576
O4 Mo2 Mo4 O9 72.7(4) . 2_576
O9 Mo2 Mo4 O9 -74.0(3) . 2_576
O6 Mo2 Mo4 O9 72.6(4) . 2_576
O10 Mo2 Mo4 O9 -75.0(3) . 2_576
O10 Mo2 Mo4 O9 -1.7(2) 2_576 2_576
Mo3 Mo2 Mo4 O9 -87.73(18) . 2_576
N3 C3 C4 C8 -105.2(13) . .
N3 C3 C4 C5 74.2(14) . .
C8 C4 C5 C6 -1.5(17) . .
C3 C4 C5 C6 179.2(11) . .
C4 C5 C6 C7 1.8(19) . .
C5 C6 C7 N4 -2(2) . .
C5 C4 C8 N4 1.8(18) . .
C3 C4 C8 N4 -178.9(10) . .
N7 C11 C12 C16 -99.8(12) . .
N7 C11 C12 C13 87.6(13) . .
C16 C12 C13 C14 2.1(16) . .
C11 C12 C13 C14 174.8(10) . .
C12 C13 C14 C15 -1.8(17) . .
C13 C14 C15 N8 1.0(17) . .
C13 C12 C16 N8 -1.6(17) . .
C11 C12 C16 N8 -174.6(10) . .
N3 C2 N1 C1 -0.4(13) . .
N3 C2 N1 Cu3 -171.9(8) . .
N2 C1 N1 C2 2.1(15) . .
N2 C1 N1 Cu3 173.7(9) . .
N8 Cu3 N1 C2 0(2) . .
O13 Cu3 N1 C2 176.9(10) . .
N8 Cu3 N1 C1 -169.6(13) . .
O13 Cu3 N1 C1 7.3(11) . .
N1 C1 N2 N3 -2.8(15) . .
N1 C2 N3 N2 -1.3(14) . .
N1 C2 N3 C3 -179.1(11) . .
C1 N2 N3 C2 2.5(13) . .
C1 N2 N3 C3 -179.5(11) . .
C4 C3 N3 C2 115.2(14) . .
C4 C3 N3 N2 -62.4(14) . .
C6 C7 N4 C8 3(2) . .
C6 C7 N4 Cu1 -169.9(10) . 2_578
C4 C8 N4 C7 -2.2(18) . .
C4 C8 N4 Cu1 170.4(9) . 2_578
N6 C9 N5 C10 -3.2(14) . .
N6 C9 N5 Cu1 176.5(8) . .
N7 C10 N5 C9 1.7(13) . .
N7 C10 N5 Cu1 -178.0(7) . .
N4 Cu1 N5 C9 2(5) 2_578 .
N4 Cu1 N5 C10 -179(100) 2_578 .
N5 C9 N6 N7 3.3(14) . .
N5 C9 N6 Cu2 -157.2(9) . .
Cl1 Cu2 N6 C9 149.9(10) . .
Cl1 Cu2 N6 C9 -34.1(11) 2_487 .
Cu2 Cu2 N6 C9 -35.9(14) 2_487 .
Cl1 Cu2 N6 N7 -5.8(17) . .
Cl1 Cu2 N6 N7 170.2(9) 2_487 .
Cu2 Cu2 N6 N7 168.4(6) 2_487 .
N5 C10 N7 N6 0.2(12) . .
N5 C10 N7 C11 170.5(9) . .
C9 N6 N7 C10 -2.0(12) . .
Cu2 N6 N7 C10 157.9(8) . .
C9 N6 N7 C11 -172.9(10) . .
Cu2 N6 N7 C11 -12.9(14) . .
C12 C11 N7 C10 118.3(12) . .
C12 C11 N7 N6 -72.5(13) . .
C14 C15 N8 C16 -0.4(16) . .
C14 C15 N8 Cu3 -174.9(8) . .
C12 C16 N8 C15 0.8(16) . .
C12 C16 N8 Cu3 175.4(8) . .
N1 Cu3 N8 C15 177.3(12) . .
O13 Cu3 N8 C15 0.4(9) . .
N1 Cu3 N8 C16 3(2) . .
O13 Cu3 N8 C16 -174.0(8) . .
O8 Mo3 O3 Mo1 70.3(5) . 2_576
O5 Mo3 O3 Mo1 178.6(4) . 2_576
O9 Mo3 O3 Mo1 -54.7(8) . 2_576
O10 Mo3 O3 Mo1 -22.4(4) . 2_576
O6 Mo3 O3 Mo1 -94.6(4) 2_576 2_576
Mo2 Mo3 O3 Mo1 -21.3(5) . 2_576
O7 Mo2 O4 Mo1 -178.8(4) . .
O9 Mo2 O4 Mo1 78.3(4) . .
O6 Mo2 O4 Mo1 -74.1(4) . .
O10 Mo2 O4 Mo1 3.2(10) . .
O10 Mo2 O4 Mo1 1.7(3) 2_576 .
Mo3 Mo2 O4 Mo1 78.6(4) . .
Mo4 Mo2 O4 Mo1 -74.2(4) . .
O1 Mo1 O4 Mo2 -4.9(18) . .
O2 Mo1 O4 Mo2 -179.8(5) . .
O3 Mo1 O4 Mo2 72.9(4) 2_576 .
O11 Mo1 O4 Mo2 -76.3(4) 2_576 .
O7 Mo2 O6 Mo4 -72.8(4) . .
O4 Mo2 O6 Mo4 -179.9(3) . .
O9 Mo2 O6 Mo4 62.1(6) . .
O10 Mo2 O6 Mo4 22.9(3) . .
O10 Mo2 O6 Mo4 100.2(3) 2_576 .
Mo3 Mo2 O6 Mo4 23.6(4) . .
O7 Mo2 O6 Mo3 172.6(3) . 2_576
O4 Mo2 O6 Mo3 65.6(4) . 2_576
O9 Mo2 O6 Mo3 -52.4(6) . 2_576
O10 Mo2 O6 Mo3 -91.6(3) . 2_576
O10 Mo2 O6 Mo3 -14.3(3) 2_576 2_576
Mo3 Mo2 O6 Mo3 -90.9(3) . 2_576
Mo4 Mo2 O6 Mo3 -114.5(4) . 2_576
O12 Mo4 O6 Mo2 73.1(4) . .
O13 Mo4 O6 Mo2 178.9(3) . .
O11 Mo4 O6 Mo2 -52.9(7) . .
O10 Mo4 O6 Mo2 -22.2(3) . .
O9 Mo4 O6 Mo2 -98.4(3) 2_576 .
O12 Mo4 O6 Mo3 -169.4(3) . 2_576
O13 Mo4 O6 Mo3 -63.7(4) . 2_576
O11 Mo4 O6 Mo3 64.6(6) . 2_576
O10 Mo4 O6 Mo3 95.2(3) . 2_576
O9 Mo4 O6 Mo3 19.1(2) 2_576 2_576
Mo2 Mo4 O6 Mo3 117.4(4) . 2_576
O7 Mo2 O9 Mo3 73.3(4) . .
O4 Mo2 O9 Mo3 179.7(3) . .
O6 Mo2 O9 Mo3 -61.9(6) . .
O10 Mo2 O9 Mo3 -22.8(3) . .
O10 Mo2 O9 Mo3 -99.9(3) 2_576 .
Mo4 Mo2 O9 Mo3 -23.6(4) . .
O7 Mo2 O9 Mo4 -172.9(3) . 2_576
O4 Mo2 O9 Mo4 -66.6(3) . 2_576
O6 Mo2 O9 Mo4 51.8(6) . 2_576
O10 Mo2 O9 Mo4 90.9(3) . 2_576
O10 Mo2 O9 Mo4 13.9(3) 2_576 2_576
Mo3 Mo2 O9 Mo4 113.7(4) . 2_576
Mo4 Mo2 O9 Mo4 90.1(3) . 2_576
O8 Mo3 O9 Mo2 -71.3(4) . .
O5 Mo3 O9 Mo2 -177.6(3) . .
O3 Mo3 O9 Mo2 54.9(6) . .
O10 Mo3 O9 Mo2 22.1(3) . .
O6 Mo3 O9 Mo2 97.4(3) 2_576 .
O8 Mo3 O9 Mo4 172.3(3) . 2_576
O5 Mo3 O9 Mo4 66.0(4) . 2_576
O3 Mo3 O9 Mo4 -61.5(6) . 2_576
O10 Mo3 O9 Mo4 -94.3(3) . 2_576
O6 Mo3 O9 Mo4 -19.0(2) 2_576 2_576
Mo2 Mo3 O9 Mo4 -116.4(4) . 2_576
O7 Mo2 O10 Mo4 81.7(3) . .
O4 Mo2 O10 Mo4 -100.3(7) . .
O9 Mo2 O10 Mo4 -179.1(3) . .
O6 Mo2 O10 Mo4 -18.8(2) . .
O10 Mo2 O10 Mo4 -98.7(3) 2_576 .
Mo3 Mo2 O10 Mo4 162.1(3) . .
O7 Mo2 O10 Mo3 -80.3(3) . .
O4 Mo2 O10 Mo3 97.6(7) . .
O9 Mo2 O10 Mo3 18.9(2) . .
O6 Mo2 O10 Mo3 179.2(3) . .
O10 Mo2 O10 Mo3 99.2(3) 2_576 .
Mo4 Mo2 O10 Mo3 -162.1(3) . .
O7 Mo2 O10 Mo2 -179.6(3) . 2_576
O4 Mo2 O10 Mo2 -1.6(9) . 2_576
O9 Mo2 O10 Mo2 -80.3(3) . 2_576
O6 Mo2 O10 Mo2 80.0(3) . 2_576
O10 Mo2 O10 Mo2 0.0 2_576 2_576
Mo3 Mo2 O10 Mo2 -99.2(3) . 2_576
Mo4 Mo2 O10 Mo2 98.7(3) . 2_576
O12 Mo4 O10 Mo2 -76.9(3) . .
O13 Mo4 O10 Mo2 94.7(9) . .
O11 Mo4 O10 Mo2 -177.3(3) . .
O6 Mo4 O10 Mo2 18.6(2) . .
O9 Mo4 O10 Mo2 93.9(3) 2_576 .
O12 Mo4 O10 Mo3 25.3(10) . .
O13 Mo4 O10 Mo3 -163.1(10) . .
O11 Mo4 O10 Mo3 -75.1(10) . .
O6 Mo4 O10 Mo3 120.8(10) . .
O9 Mo4 O10 Mo3 -163.9(10) 2_576 .
Mo2 Mo4 O10 Mo3 102.2(10) . .
O12 Mo4 O10 Mo2 177.7(3) . 2_576
O13 Mo4 O10 Mo2 -10.7(10) . 2_576
O11 Mo4 O10 Mo2 77.3(3) . 2_576
O6 Mo4 O10 Mo2 -86.8(3) . 2_576
O9 Mo4 O10 Mo2 -11.6(2) 2_576 2_576
Mo2 Mo4 O10 Mo2 -105.4(3) . 2_576
O8 Mo3 O10 Mo2 77.3(3) . .
O5 Mo3 O10 Mo2 -90.6(10) . .
O3 Mo3 O10 Mo2 178.7(3) . .
O9 Mo3 O10 Mo2 -18.6(2) . .
O6 Mo3 O10 Mo2 -93.5(3) 2_576 .
O8 Mo3 O10 Mo4 -25.0(10) . .
O5 Mo3 O10 Mo4 167.2(10) . .
O3 Mo3 O10 Mo4 76.4(10) . .
O9 Mo3 O10 Mo4 -120.9(10) . .
O6 Mo3 O10 Mo4 164.3(10) 2_576 .
Mo2 Mo3 O10 Mo4 -102.3(10) . .
O8 Mo3 O10 Mo2 -177.3(3) . 2_576
O5 Mo3 O10 Mo2 14.8(11) . 2_576
O3 Mo3 O10 Mo2 -75.9(3) . 2_576
O9 Mo3 O10 Mo2 86.8(3) . 2_576
O6 Mo3 O10 Mo2 11.9(2) 2_576 2_576
Mo2 Mo3 O10 Mo2 105.4(3) . 2_576
O12 Mo4 O11 Mo1 -75.0(5) . 2_576
O13 Mo4 O11 Mo1 178.3(4) . 2_576
O6 Mo4 O11 Mo1 50.0(8) . 2_576
O10 Mo4 O11 Mo1 20.0(4) . 2_576
O9 Mo4 O11 Mo1 92.7(4) 2_576 2_576
Mo2 Mo4 O11 Mo1 17.8(5) . 2_576
O12 Mo4 O13 Cu3 -55(2) . .
O11 Mo4 O13 Cu3 50.1(19) . .
O6 Mo4 O13 Cu3 -154.6(18) . .
O10 Mo4 O13 Cu3 134.1(15) . .
O9 Mo4 O13 Cu3 134.9(19) 2_576 .
Mo2 Mo4 O13 Cu3 -153.7(17) . .
N1 Cu3 O13 Mo4 61.7(19) . .
N8 Cu3 O13 Mo4 -119.2(19) . .
N6 Cu2 Cl1 Cu2 176.1(10) . 2_487
Cl1 Cu2 Cl1 Cu2 0.0 2_487 2_487
